Polyurethane (PUR and PU) is a polymer composed of a chain of organic units joined by carbamate (urethane) links. While most polyurethanes are thermosetting polymers that do not melt when heated, thermoplastic polyurethanes are also available.
Polyurethane products often are simply called “urethanes”, but should not be confused with ethyl carbamate, which is also called urethane. Polyurethanes neither contain nor are produced from ethyl carbamate.
Polyurethanes are used in the manufacture of flexible, high-resilience foam seating; rigid foam insulation panels; microcellular foam seals and gaskets; durable elastomeric wheels and tires (such as roller coaster wheels); automotive suspension bushings; electrical potting compounds; high performance adhesives; surface coatings and surface sealants; synthetic fibers (e.g., Spandex); carpet underlay; hard-plastic parts (e.g., for electronic instruments); hoses and skateboard wheels.
Otto Bayer and his coworkers at I.G. Farben in Leverkusen, Germany, first made polyurethanes in 1937. The new polymers had some advantages over existing plastics that were made by polymerizing olefins, or by polycondensation, and were not covered by patents obtained by Wallace Carothers on polyesters. Early work focused on the production of fibres and flexible foams and PUs were applied on a limited scale as aircraft coating during World War II. Polyisocyanates became commercially available in 1952 and production of flexible polyurethane foam began in 1954 using toluene diisocyanate (TDI) and polyester polyols. These materials were also used to produce rigid foams, gum rubber, and elastomers. Linear fibers were produced from hexamethylene diisocyanate (HDI) and 1,4-butanediol (BDO).
In 1956 DuPont introduced polyether polyols, specifically poly(tetramethylene ether) glycol and BASF and Dow Chemical started selling polyalkylene glycols in 1957. Polyether polyols were cheaper, easier to handle and more water resistant than polyester polyols, and became more popular. Union Carbide and Mobay, a U.S. Monsanto/Bayer joint venture, also began making polyurethane chemicals. In 1960 more than 45,000 metric tons of flexible polyurethane foams were produced. The availability of chlorofluoroalkane blowing agents, inexpensive polyether polyols, and methylene diphenyl diisocyanate (MDI) allowed polyurethane rigid foams to be used as high performance insulation materials. In 1967, urethane modified polyisocyanurate rigid foams were introduced, offering even better thermal stability and flammability resistance. During the 1960s, automotive interior safety components such as instrument and door panels were produced by back-filling thermoplastic skins with semi-rigid foam.
In 1969, Bayer exhibited an all plastic car in Düsseldorf, Germany. Parts of this car, such as the fascia and body panels were manufactured using a new process called RIM, Reaction Injection Molding in which the reactants were mixed then injected into a mold. The addition of fillers, such as milled glass, mica, and processed mineral fibres gave rise to reinforced RIM (RRIM), which provided improvements in flexural modulus (stiffness), reduction in coefficient of thermal expansion and thermal stability. This technology was used to make the first plastic-body automobile in the United States, the Pontiac Fiero, in 1983. Further increases in stiffness were obtained by incorporating pre-placed glass mats into the RIM mold cavity, also known broadly as resin injection molding or structural RIM.
Starting in the early 1980s, water-blown microcellular flexible foams were used to mold gaskets for automotive panels and air filter seals, replacing PVC plastisol from automotive applications have greatly increased market share. Polyurethane foams are now used in high temperature oil filter applications.
Polyurethane foam (including foam rubber) is sometimes made using small amounts of blowing agents to give less dense foam, better cushioning/energy absorption or thermal insulation. In the early 1990s, because of their impact on ozone depletion, the Montreal Protocol restricted the use of many chlorine-containing blowing agents, such as trichlorofluoromethane (CFC-11). By the late 1990s, the use of blowing agents such as carbon dioxide, pentane, 1,1,1,2-tetrafluoroethane (HFC-134a) and 1,1,1,3,3-pentafluoropropane (HFC-245fa) were widely used in North America and the EU, although chlorinated blowing agents remained in use in many developing countries.
In the 1990s new two-component polyurethane and hybrid polyurethane-polyurea elastomers were used for spray-in-place load bed liners and military marine applications for the U.S. Navy. A one-part polyurethane is specified as high durability deck coatings under MIL-PRF-32171 for the US Navy. This technique for coating creates a durable, abrasion resistant composite with the metal substrate, and eliminates corrosion and brittleness associated with drop-in thermoplastic bed liners.
Rising costs of petrochemical feedstocks and an enhanced public desire for environmentally friendly green products raised interest in polyols derived from vegetable oils. One of the most vocal supporters of these polyurethanes made using natural oil polyols is the Ford Motor Company.
Polyurethanes are in the class of compounds called reaction polymers, which include epoxies, unsaturated polyesters, and phenolics. Polyurethanes are produced by reacting an isocyanate containing two or more isocyanate groups per molecule (R-(N=C=O)n ≥ 2) with a polyol containing on average two or more hydroxy groups per molecule (R'-(OH)n ≥ 2), in the presence of a catalyst.
The properties of a polyurethane are greatly influenced by the types of isocyanates and polyols used to make it. Long, flexible segments, contributed by the polyol, give soft, elastic polymer. High amounts of crosslinking give tough or rigid polymers. Long chains and low crosslinking give a polymer that is very stretchy, short chains with lots of crosslinks produce a hard polymer while long chains and intermediate crosslinking give a polymer useful for making foam. The crosslinking present in polyurethanes means that the polymer consists of a three-dimensional network and molecular weight is very high. In some respects a piece of polyurethane can be regarded as one giant molecule. One consequence of this is that typical polyurethanes do not soften or melt when they are heated...they are thermosetting polymers. The choices available for the isocyanates and polyols, in addition to other additives and processing conditions allow polyurethanes to have the very wide range of properties that make them such widely used polymers.
Isocyanates are very reactive materials. This makes them useful in making polymers but also requires special care in handling and use. The aromatic isocyanates, diphenylmethane diisocyanate (MDI) or toluene diisocyanate (TDI) are more reactive than aliphatic isocyanates, such as hexamethylene diisocyanate (HDI) or isophorone diisocyanate (IPDI). Most of the isocyanates are difunctional, that is they have exactly two isocyanate groups per molecule. An important exception to this is polymeric diphenylmethane diisocyanate, which is a mixture of molecules with two-, three-, and four- or more isocyanate groups. In cases like this the material has an average functionality greater than two, commonly 2.7. Isocyanates with functionality greater than two act as crosslinking sites as mentioned in the previous paragraph.
Polyols are polymers in their own right and have on average two or more hydroxyl groups per molecule. Polyether polyols are mostly made by polymerizing ethylene oxide and propylene oxide. Polyester polyols are made similarly to polyester polymers. The polyols used to make polyurethanes are not "pure" compounds since they are often mixtures of similar molecules with different molecular weights and mixtures of molecules that contain different numbers of hydroxyl groups, which is why the "average functionality" is often mentioned. Despite them being complex mixtures, industrial grade polyols have their composition sufficiently well controlled to produce polyurethanes having consistent properties. As mentioned earlier, it is the length of the polyol chain and the functionality that contribute much to the properties of the final polymer. Polyols used to make rigid polyurethanes have molecular weights in the hundreds, while those used to make flexible polyurethanes have molecular weights up to ten thousand or more.
|PU reaction mechanism catalyzed by a tertiary amine|
|generalized urethane reaction|
The polymerization reaction makes a polymer containing the urethane linkage, -RNHCOOR'- and is catalyzed by tertiary amines, such as 1,4-diazabicyclo[2.2.2]octane (also called DABCO or TEDA), and metallic compounds, such as dibutyltin dilaurate or bismuth octanoate. This is often referred to as the gellation reaction or simply gelling.
If water is present in the reaction mixture (it is often added intentionally to make foams), the isocyanate reacts with water to form a urea linkage and carbon dioxide gas and the resulting polymer contains both urethane and urea linkages. This reaction is referred to as the blowing reaction and is catalyzed by tertiary amines like bis-(2-dimethylaminoethyl)ether.
One of the most desirable attributes of polyurethanes is their ability to be turned into foam. Making a foam requires the formation of a gas at the same time as the urethane polymerization (gellation) is occurring. The gas can be carbon dioxide, either generated by reacting isocyanate with water. or added as a gas or produced by boiling volatile liquids. In the latter case heat generated by the polymerization causes the liquids to vaporize. The liquids can be HFC-245fa (1,1,1,3,3-pentafluoropropane) and HFC-134a (1,1,1,2-tetrafluoroethane), and hydrocarbons such as n-pentane.
|carbon dioxide gas formed by reacting water and isocyanate|
When water is used to produce the gas, care must be taken to use the right combination of catalysts to achieve the proper balance between gellation and blowing. The reaction to generate carbon dioxide involves water molecule reacting with an isocyanate first forming an unstable carbamic acid, which then decomposes into carbon dioxide and an amine. The amine reacts with more isocyanate to give a substituted urea. Water has a very low molecular weight, so even though the weight percent of water may be small, the molar proportion of water may be high and considerable amounts of urea produced. The urea is not very soluble in the reaction mixture and tends to form separate "hard segment" phases consisting mostly of polyurea. The concentration and organization of these polyurea phases can have a significant impact on the properties of the polyurethane foam.
High-density microcellular foams can be formed without the addition of blowing agents by mechanically frothing or nucleating the polyol component prior to use.
Surfactants are used in polyurethane foams to emulsify the liquid components, regulate cell size, and stabilize the cell structure to prevent collapse and surface defects. Rigid foam surfactants are designed to produce very fine cells and a very high closed cell content. Flexible foam surfactants are designed to stabilize the reaction mass while at the same time maximizing open cell content to prevent the foam from shrinking.
An even more rigid foam can be made with the use of specialty trimerization catalysts which create cyclic structures within the foam matrix, giving a harder, more thermally stable structure, designated as polyisocyanurate foams. Such properties are desired in rigid foam products used in the construction sector.
Careful control of viscoelastic properties — by modifying the catalysts and polyols used —can lead to memory foam, which is much softer at skin temperature than at room temperature.
Foams can be either "closed cell", where most of the original bubbles or cells remain intact, or "open cell", where the bubbles have broken but the edges of the bubbles are stiff enough to retain their shape. Open cell foams feel soft and allow air to flow through so they are comfortable when used in seat cushions or mattresses. Closed cell rigid foams are used as thermal insulation, for example in refrigerators.
Raw materials 
Isocyanates used to make polyurethane must have two or more isocyanate groups on each molecule. The most commonly used isocyanates are the aromatic diisocyantes, toluene diisocyanate (TDI) and methylene diphenyl diisocyanate, MDI.
TDI and MDI are generally less expensive and more reactive than other isocyanates. Industrial grade TDI and MDI are mixtures of isomers and MDI often contains polymeric materials. They are used to make flexible foam (for example slabstock foam for mattresses or molded foams for car seats), rigid foam (for example insulating foam in refrigerators) elastomers (shoe soles, for example), and so on. The isocyanates may be modified by partially reacting them with polyols or introducing some other materials to reduce volatility (and hence toxicity) of the isocyanates, decrease their freezing points to make handling easier or to improve the properties of the final polymers.
Aliphatic and cycloaliphatic isocyanates are used in smaller volumes, most often in coatings and other applications where color and transparency are important since polyurethanes made with aromatic isocyanates tend to darken on exposure to light. The most important aliphatic and cycloaliphatic isocyanates are 1,6-hexamethylene diisocyanate (HDI), 1-isocyanato-3-isocyanatomethyl-3,5,5-trimethyl-cyclohexane (isophorone diisocyanate, IPDI), and 4,4'-diisocyanato dicyclohexylmethane, (H12MDI or hydrogenated MDI).
Polyols can be polyether polyols, which are made by the reaction of epoxides with an active hydrogen containing starter compounds, or polyester polyols, which are made by the polycondensation of multifunctional carboxylic acids and hydroxyl compounds. They can be further classified according to their end use. Higher molecular weight polyols (molecular weights from 2,000 to 10,000) are used to make more flexible polyurethanes while lower molecular weight polyols make more rigid products.
Polyols for flexible applications use low functionality initiators such as dipropylene glycol (f=2), glycerine (f=3) or a sorbitol/water solution (f=2.75). Polyols for rigid applications use high functionality initiators such as sucrose (f=8), sorbitol (f=6), toluenediamine (f=4), and Mannich bases (f=4). Propylene oxide and/or ethylene oxide is added to the initiators until the desired molecular weight is achieved. The order of addition and the amounts of each oxide affect many polyol properties, such as compatibility, water-solubility, and reactivity. Polyols made with only propylene oxide are terminated with secondary hydroxyl groups and are less reactive than polyols capped with ethylene oxide, which contain a higher percentage of primary hydroxyl groups. Graft polyols (also called filled polyols or polymer polyols) contain finely dispersed styrene-acrylonitrile, acrylonitrile, or polyurea (PHD) polymer solids chemically grafted to a high molecular weight polyether backbone. They are used to increase the load-bearing properties of low-density high-resiliency (HR) foam, as well as add toughness to microcellular foams and cast elastomers. Initiators such as ethylenediamine and triethanolamine are used to make low molecular weight rigid foam polyols that have built-in catalytic activity due to the presence of nitrogen atoms in the backbone. A special class of polyether polyols, poly(tetramethylene ether) glycols, which are made by polymerizing tetrahydrofuran, are used in high performance coating, wetting and elastomer applications.
Conventional polyester polyols are based on virgin raw materials and are manufactured by the direct polyesterification of high-purity diacids and glycols, such as adipic acid and 1,4-butanediol. Polyester polyols are usually more expensive and more viscous than polyether polyols, but they make polyurethanes with better solvent, abrasion, and cut resistance. Other polyester polyols are based on reclaimed raw materials. They are manufactured by transesterification (glycolysis) of recycled poly(ethyleneterephthalate) (PET) or dimethylterephthalate (DMT) distillation bottoms with glycols such as diethylene glycol. These low molecular weight, aromatic polyester polyols are used in rigid foam, and bring low cost and excellent flammability characteristics to polyisocyanurate (PIR) boardstock and polyurethane spray foam insulation.
Specialty polyols include polycarbonate polyols, polycaprolactone polyols, polybutadiene polyols, and polysulfide polyols. The materials are used in elastomer, sealant, and adhesive applications that require superior weatherability, and resistance to chemical and environmental attack. Natural oil polyols derived from castor oil and other vegetable oils are used to make elastomers, flexible bunstock, and flexible molded foam. Copolymerizing chlorotrifluoroethylene or tetrafluoroethylene with vinyl ethers containing hydroxyalkyl vinyl ether produces fluorinated (FEVE) polyols. Two component fluorinated polyurethane prepared by reacting FEVE fluorinated polyols with polyisocyanate have been applied for make ambient cure paint/coating. Since fluorinated polyurethanes contain high percentage of fluorine-carbon bond which is the strongest bond among all chemical bonds. Fluorinated polyurethanes have excellent resistance to UV, acids, alkali, salts, chemicals, solvents, weathering, corrosion, fungi and microbial attack. These have become the first choice for high performance coating/paints.
Chain extenders (f=2) and cross linkers (f=3 or greater) are low molecular weight hydroxyl and amine terminated compounds that play an important role in the polymer morphology of polyurethane fibers, elastomers, adhesives, and certain integral skin and microcellular foams. The elastomeric properties of these materials are derived from the phase separation of the hard and soft copolymer segments of the polymer, such that the urethane hard segment domains serve as cross-links between the amorphous polyether (or polyester) soft segment domains. This phase separation occurs because the mainly non-polar, low melting soft segments are incompatible with the polar, high melting hard segments. The soft segments, which are formed from high molecular weight polyols, are mobile and are normally present in coiled formation, while the hard segments, which are formed from the isocyanate and chain extenders, are stiff and immobile. Because the hard segments are covalently coupled to the soft segments, they inhibit plastic flow of the polymer chains, thus creating elastomeric resiliency. Upon mechanical deformation, a portion of the soft segments are stressed by uncoiling, and the hard segments become aligned in the stress direction. This reorientation of the hard segments and consequent powerful hydrogen bonding contributes to high tensile strength, elongation, and tear resistance values. The choice of chain extender also determines flexural, heat, and chemical resistance properties. The most important chain extenders are ethylene glycol, 1,4-butanediol (1,4-BDO or BDO), 1,6-hexanediol, cyclohexane dimethanol and hydroquinone bis(2-hydroxyethyl) ether (HQEE). All of these glycols form polyurethanes that phase separate well and form well defined hard segment domains, and are melt processable. They are all suitable for thermoplastic polyurethanes with the exception of ethylene glycol, since its derived bis-phenyl urethane undergoes unfavorable degradation at high hard segment levels. Diethanolamine and triethanolamine are used in flex molded foams to build firmness and add catalytic activity. Diethyltoluenediamine is used extensively in RIM, and in polyurethane and polyurea elastomer formulations.
|hydroxyl compounds – difunctional molecules|
|MW||s.g.||m.p. °C||b.p. °C|
|hydroxyl compounds – trifunctional molecules|
|MW||s.g.||f.p. °C||b.p. °C|
|hydroxyl compounds – tetrafunctional molecules|
|MW||s.g.||m.p. °C||b.p. °C|
|amine compounds – difunctional molecules|
|MW||s.g.||m.p. °C||b.p. °C|
Polyurethane catalysts can be classified into two broad categories, amine compounds and metal complexes. Traditional amine catalysts have been tertiary amines such as triethylenediamine (TEDA, 1,4-diazabicyclo[2.2.2]octane or DABCO), dimethylcyclohexylamine (DMCHA), and dimethylethanolamine (DMEA). Tertiary amine catalysts are selected based on whether they drive the urethane (polyol+isocyanate, or gel) reaction, the urea (water+isocyanate, or blow) reaction, or the isocyanate trimerization reaction (e.g., using potassium acetate, to form isocyanurate ring structure). Catalysts that contain a hydroxyl group or secondary amine, which react into the polymer matrix, can replace traditional catalysts thereby reducing the amount of amine that can come out of the polymer.
Metallic compounds based on mercury, lead, tin, bismuth, and zinc are used as polyurethane catalysts. Mercury carboxylates, are particularly effective catalysts for polyurethane elastomer, coating and sealant applications, since they are very highly selective towards the polyol+isocyanate reaction, but they are toxic. Bismuth and zinc carboxylates have been used as alternatives. Alkyl tin carboxylates, oxides and mercaptides oxides are used in all types of polyurethane applications. Tin mercaptides are used in formulations that contain water, as tin carboxylates are susceptible to hydrolysis.
Surfactants are used to modify the characteristics of both foam and non-foam polyurethane polymers. They take the form of polydimethylsiloxane-polyoxyalkylene block copolymers, silicone oils, nonylphenol ethoxylates, and other organic compounds. In foams, they are used to emulsify the liquid components, regulate cell size, and stabilize the cell structure to prevent collapse and sub-surface voids. In non-foam applications they are used as air release and anti-foaming agents, as wetting agents, and are used to eliminate surface defects such as pin holes, orange peel, and sink marks.
Polyurethanes are produced by mixing two or more liquid streams. The isocyanate is usually added by itself and the polyol stream is usually more complex, containing catalysts, surfactants, blowing agents and so on. The two components are referred to as a polyurethane system, or simply a system. The isocyanate is commonly referred to in North America as the 'A-side' or just the 'iso'. The blend of polyols and other additives is commonly referred to as the 'B-side' or as the 'poly'. This mixture might also be called a 'resin' or 'resin blend'. In Europe the meanings for 'A-side' and 'B-side' are reversed. Resin blend additives may include chain extenders, cross linkers, surfactants, flame retardants, blowing agents, pigments, and fillers. Polyurethane can be made in a variety of densities and hardnesses by varying the isocyanate, polyol or additives.
Health and safety 
Fully reacted polyurethane polymer is chemically inert. No exposure limits have been established by OSHA (Occupational Safety and Health Administration) or ACGIH (American Conference of Governmental Industrial Hygienists). It is not regulated by OSHA for carcinogenicity. Polyurethane polymer is a combustible solid and can be ignited if exposed to an open flame. Decomposition from fire can produce mainly carbon monoxide, and trace nitrogen oxides and hydrogen cyanide. Firefighters should wear self-contained breathing apparatus in enclosed areas.
Liquid resin blends and isocyanates may contain hazardous or regulated components. They should be handled in accordance with manufacturer recommendations found on product labels, and in MSDS (Material Safety Data Sheet) and product technical literature. Isocyanates are known skin and respiratory sensitizers, and proper engineering controls should be in place to prevent exposure to isocyanate liquid and vapor. Additionally, amines, glycols, and phosphate present in spray polyurethane foams present unknown risks to the individuals exposed to them. Proper hygiene controls and personal protective equipment (PPE), such as gloves, respirators, and protective clothing and eye wear should be used.
In the United States, additional health and safety information can be found through organizations such as the Polyurethane Manufacturers Association (PMA) and the Center for the Polyurethanes Industry (CPI), as well as from polyurethane system and raw material manufacturers. In Europe, health and safety information is available from ISOPA, the European Diisocyanate and Polyol Producers Association. Regulatory information can be found in the Code of Federal Regulations Title 21 (Food and Drugs) and Title 40 (Protection of the Environment).
The methods of manufacturing polyurethane finished goods range from small, hand pour piece-part operations to large, high-volume bunstock and boardstock production lines. Regardless of the end-product, the manufacturing principle is the same: to meter the liquid isocyanate and resin blend at a specified stoichiometric ratio, mix them together until a homogeneous blend is obtained, dispense the reacting liquid into a mold or on to a surface, wait until it cures, then demold the finished part.
Dispensing equipment 
Although the capital outlay can be high, it is desirable to use a meter-mix or dispense unit for even low-volume production operations that require a steady output of finished parts. Dispense equipment consists of material holding (day) tanks, metering pumps, a mix head, and a control unit. Often, a conditioning or heater-chiller unit is added to control material temperature in order to improve mix efficiency, cure rate, and to reduce process variability. Choice of dispense equipment components depends on shot size, throughput, material characteristics such as viscosity and filler content, and process control. Material day tanks may be single to hundreds of gallons in size, and may be supplied directly from drums, IBCs (intermediate bulk containers, such as totes), or bulk storage tanks. They may incorporate level sensors, conditioning jackets, and mixers. Pumps can be sized to meter in single grams per second up to hundreds of pounds per minute. They can be rotary, gear, or piston pumps, or can be specially hardened lance pumps to meter liquids containing highly abrasive fillers such as wollastonite, chopped or hammer milled glass fibres.
The pumps can drive low-pressure (10 to 30 bar, ~1 to 3 MPa) or high-pressure (125 to 250 bar, ~12.5 to 25.0 MPa) dispense systems. Mix heads can be simple static mix tubes, rotary element mixers, low-pressure dynamic mixers, or high-pressure hydraulically actuated direct impingement mixers. Control units may have basic on/off – dispense/stop switches, and analogue pressure and temperature gauges, or may be computer controlled with flow meters to electronically calibrate mix ratio, digital temperature and level sensors, and a full suite of statistical process control software. Add-ons to dispense equipment include nucleation or gas injection units, and third or fourth stream capability for adding pigments or metering in supplemental additive packages.
Distinct from pour-in-place, bun and boardstock, and coating applications, the production of piece parts requires some type of tooling to contain and form the reacting liquid. The choice of mold-making material is dependent on the expected number of uses to end-of-life (EOL), molding pressure, flexibility, and heat transfer characteristics.
RTV silicone is used for tooling that has an EOL in the thousands of parts. It is typically used for molding rigid foam parts, where the ability to stretch and peel the mold around undercuts is needed. The heat transfer characteristic of RTV silicone tooling is poor. High-performance, flexible polyurethane elastomers are also used in this way.
Epoxy, metal-filled epoxy, and metal-coated epoxy is used for tooling that has an EOL in the tens-of-thousands of parts. It is typically used for molding flexible foam cushions and seating, integral skin and microcellular foam padding, and shallow-draft RIM bezels and fascia. The heat transfer characteristic of epoxy tooling is fair; the heat transfer characteristic of metal-filled and metal-coated epoxy is good. Copper tubing can be incorporated into the body of the tool, allowing hot water to circulate and heat the mold surface.
Aluminum is used for tooling that has an EOL in the hundreds-of-thousands of parts. It is typically used for molding microcellular foam gasketing and cast elastomer parts, and is milled or extruded into shape.
Mirror-finish stainless steel is used for tooling that imparts a glossy appearance to the finished part. The heat transfer characteristic of metal tooling is excellent.
Finally, molded or milled polypropylene is used to create low-volume tooling for molded gasket applications. Instead of many expensive metal molds, low-cost plastic tooling can be formed from a single metal master, which also allows greater design flexibility. The heat transfer characteristic of polypropylene tooling is poor, which must be taken into consideration during the formulation process.
In 2007, the global consumption of polyurethane raw materials was above 12 million metric tons, the average annual growth rate is about 5%.
Effects of visible light 
Polyurethanes, especially those made using aromatic isocyanates, contain chromophores which interact with light. This is of particular interest in the area of polyurethane coatings, where light stability is a critical factor and is the main reason that aliphatic isocyanates are used in making polyurethane coatings. When PU foam, which is made using aromatic isocyanates, is exposed to visible light it discolors, turning from off-white to yellow to reddish brown. It has been generally accepted that apart from yellowing, visible light has little effect on foam properties. This is especially the case if the yellowing happens on the outer portions of a large foam, as the deterioration of properties in the outer portion has little effect on the overall bulk properties of the foam itself.
It has been reported that exposure to visible light can affect the variability of some physical property test results. Consequently, it was recommended that foam samples should be protected from exposure to light prior to testing.
See also 
- Thermoplastic polyurethanes
- Passive fire protection
- Penetrant (mechanical, electrical, or structural)
- Otto Bayer "Das Di-Isocyanat-Polyadditionsverfahren (Polyurethane)" Angewandte Chemie, 1947, Volume 59, pages 257–272. doi:10.1002/ange.19470590901. See also German Patent 728.981 (1937) I.G. Farben
- Polyurethanes: A Class of Modern Versatile Materials Raymond B. Seymour George B. Kauffman J. Chem. Ed. 69, 909 1992
- Feske, Bert (October 2004). "The Use of Saytex RB-9130/9170 Low Viscosity Brominated Flame Retardant Polyols in HFC-245fa and High Water Formulations". Las Vegas, NV: Alliance for the Polyurethane Industry Technical Conference.
- NST Center. (2010).  ”Mil Specs for High Durability Deck Coatings (Mil-prf-32171) Durabak-M26”
- Niemeyer, Timothy; Patel, Munjal and Geiger, Eric (September, 2006). "A Further Examination of Soy-Based Polyols in Polyurethane Systems". Salt Lake City, UT: Alliance for the Polyurethane Industry Technical Conference.
- "New Twist on Green: 2008 Ford Mustang Seats Will Be Soy-Based Foam". Edmunds inside line. July 12, 2007. Archived from the original on 2008-05-31. Retrieved 2010-06-15.
- Gum, Wilson; Riese, Wolfram; Ulrich, Henri (1992). Reaction Polymers. New York: Oxford University Press. ISBN 0-19-520933-8.
- Harrington, Ron; Hock, Kathy (1991). Flexible Polyurethane Foams. Midland: The Dow Chemical Company.
- Oertel, Gunter (1985). Polyurethane Handbook. New York: Macmillen Publishing Co., Inc. ISBN 0-02-948920-2.
- Ulrich, Henri (1996). Chemistry and Technology of Isocyanates. New York: John Wiley & Sons, Inc. ISBN 0-471-96371-2.
- Woods, George (1990). The ICI Polyurethanes Book. New York: John Wiley & Sons, Inc. ISBN 0-471-92658-2.
- Kaushiva, Byran D. (August 15, 1999). Structure-Property Relationships of Flexible Polyurethane Foams. PhD Thesis. Virginia Polytechnic Institute.
- "Technical data sheet from Dow Chemical". Retrieved 2007-09-15.
- Randall, David; Lee, Steve (2002). The Polyurethanes Book. New York: Wiley. ISBN 0-470-85041-8.
- Blackwell, J.; M.R. Nagarajan and T.B. Hoitink (1981). The Structure of the Hard Segments in MDI/diol/PTMA Polyurethane Elastomers. Washington, D.C.: American Chemical Society. ISSN 0097-6156/81/0172-0179.
- Blackwell, John; Kenncorwin H. Gardner (1979). Structure of the hard segments in polyurethane elastomers. IPC Business Press. ISSN 0032-3861/79/010013-05.
- Grillo, D.J.; Housel, T.L. (1992). "Physical Properties of Polyurethanes from Polyesters and Other Polyols". Polyurethanes '92 Conference Proceedings. New Orleans, LA: The Society of the Plastics Industry, Inc..
- Musselman, S.G.; Santosusso, T.M. and Sperling, L.H. (1998). "Structure Versus Performance Properties of Cast Elastomers". Polyurethanes '98 Conference Proceedings. Dallas, TX: The Society of the Plastics Industry, Inc..
- "A Guide To Glycols". 117-00991-92HYC (The Dow Chemical Company). 1992.
- "Jeffcat Amine Catalysts for the Polyurethane Industry" (pdf). 2006. Archived from the original on 2007-11-29. Retrieved 2007-10-23.
- "Building quality with Air Products trimerisation catalysts" (pdf). 2003. Retrieved 2007-10-23.
- "FOMREZ Specialty Tin Catalysts for Polyurethane Applications". 120-074-10 (Crompton Corporation). 2001-01.
- "FOMREZ Specialty Tin Catalysts for Polyurethane Applications (leaflet insert)". 120-075-10 (Crompton Corporation). 2001-01.
- Dernehl CU. (1966). Health Hazards Associated with Polyurethane. Journal of Occupational and Environmental Medicine.
- Health Alert: Polyurethane exposure.
- CDC - NIOSH Science Blog - Help Wanted: Spray Polyurethane Foam Insulation Research.
- http://www.isopa.org ISOPA
- Fungus that eats plastic discovered Positive News 05 MAR 2012
- G. Avar, Polyurethanes (PU), Kunststoffe international 10/2008, 123-127.
- "Discoloration of polyurethane foam". Foamex Information sheet. Archived from the original on 2010-09-26. Retrieved 2010-09-26.
- Valentine, C; Craig, T.A.; Hager, S.L (1993). "Inhibition of the Discoloration of Polyurethane Foam Caused by Ultraviolet Light". J. Cellular Plastics 29 (6): 569–590. doi:10.1177/0021955X9302900605.
- Blair, G. Ron; Bob Dawe, Jim McEvoy, Roy Pask, Marcela Rusan de Priamus, Carol Wright (2007). "The Effect of Visible Light on the Variability of Flexible Foam Compression Sets". Orlando, Florida: Center for the Polyurethane Industry.
- Newman, C.R.; Forciniti, D. (2001). "Modeling the Ultraviolet Photodegradation of Rigid Polyurethane Foams". Ind. Eng. Chem. Res. 40 (15): 3336–3352. doi:10.1021/ie0009738.
|Wikimedia Commons has media related to: Polyurethane foam|
- Center for the Polyurethanes Industry: information for EH&S issues related to polyurethanes developments
- Polyurethane synthesis, Polymer Science Learning Center, University of Southern Mississippi
- Polyurethane Foam Association: Industry information, educational materials and resources related to flexible polyurethane foam
- European PU insulation industry association: (Formerly BING) European voice for the National trade associations representing the polyurethane insulation industry.